INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS


 Marjory Cox
 1 years ago
 Views:
Transcription
1 ISSN (Print), ISSN (Online) ID: TG Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko KNEZIĆ Abstract: Poisson's ratio is one of the fundamental properties of any structural material including woven fabrics and textile materials. This coefficient determines important mechanical characteristics of fabrics in many applications, including a variety of composite systems containing textiles as a structural element. Due to the anisotropy of woven fabrics, Poisson's ratio changes over the fabric sample stretching. In this paper, the practical application of the uniaxial testing of woven fabrics for determining its breaking properties and Poisson's ratio is presented. Experimental testing was carried out on two different fabrics of a different raw material composition (, ) and of the same weave (plain weave). Samples were stretched with tensile force in the weft and warp direction, and based on the different measured values of the fabric stretching, warp and weft, Poisson's ratio is calculated. The influence of the raw material composition on the values of Poisson's ratio was examined. Keywords: anisotropy; elongation at break; Poisson s ratio; warp; weft; woven fabric 1 INTRODUCTION Nowadays, the use of textile materials in different industrial branches is on the rise. Anisotropy is a characteristic of most materials, especially woven fabrics. The impact of the direction of action of the external load (tensile force) on the properties of the fabric is enormous, and is frequently examined [1]. The mechanical properties of fabrics under the influence of the tensile load began to be studied in 1937 [2]. Kilby defined the Poisson's ratio and measured the tensile properties of fabrics in an arbitrary direction of the tensile force. He noted that there is a connection between the Poisson's ratio, shear modulus and modulus of the elasticity of the fabric [3]. The Poisson's ratio affects certain mechanical properties of the fabric such as the draping and shear. The researchers determined Poisson's ratio in the warp and weft based on the geometric model of fabric and without the impact of the Poisson's ratio of the yarn. The Poisson's ratio in fabrics comes out of the interaction between the warp and weft, and can be expressed in terms of structural and mechanical system parameters [4]. Due to the woven fabric anisotropy, the analysis of the impact of the physical parameters of fabric on the value of the Poisson's ratio is useful and provides a better explanation for certain woven fabric behavior. Because of the inherent nature of textile, an accurate and reliable measurement of the Poisson's ratio is a difficult task. This engineering property is studied by many scientists. Bao and colleagues [5] were examining why in the measurements of the Poisson's ratio, when uniaxial tensile load is put on the fabric, errors occur. The previously measured experimental values were compared with the theoretical results. He also studied the influence of the yarn and fabric structural parameters of the Poisson's ratio. An accurate measurement of the Poisson's ratio of woven fabric is quite difficult to obtain due to the lack of reliable experimental techniques [6]. Uniaxial testing is most commonly performed in woven fabrics by using either the commercial or custom designed instruments [7] and analyzing the physical and mechanical properties of textile products [8]. The Poisson's ratio of textile materials used in the nonwoven geotextile was analyzed by Giroud [9]. He set the theoretical equation to calculate the Poisson coefficient, as a function of strain. Experiments on the extension of the woven fabric sample under the static load will are discussed in this paper. The influence of the raw material composition on the values of the Poisson's ratio has been researched, too. 2 THEORETICAL OVERVIEW The Poisson's ratio, which expresses the change in the volume of a solid undergoing deformation, is an important characteristic, along with the initial modulus of elasticity and shear, of the behavior of a material under a tension load; and can be used in the calculations of the true stresses (from the actual crosssectional area) coming into being in the textile fibers and yarns subjected to the extension, and can serve, moreover, as an indirect characteristic of the structure of the material and of the mechanism of its deformation. It is well known that when a solid having the shape of a rectangular parallelepiped, Fig. 1a, is subjected to tension forces in the direction of its axes x, y and z, the change in its volume equals: dv y z d x x z d y x y d V x y z d d x y d z x y z x y z where ε x, ε y and ε z are the relative tensile deformations in the direction of the x, y and z axes of the parallelepiped. z (1) TEHNIČKI GLASNIK 11, 3(217),
2 dx L z dy s y (1+ y )dy L d x x T (1+ y )d y s x s x d y T y s y (1+ x )dx (1+ x )d x a) b) c) Figure 1 Schematic presentation of: a) solid volume element, b) Poisson s ratio ν xy, c) Poisson s ratio ν yx In the tensile deformation in the direction of the x axis, the solid will be subjected to compression in the direction of the y and z axes (i.e, laterally to the x axis): dv V x 2 x 1 2 x 1 2 x where ε is the relative compressive deformation and ν is the Poisson s ratio. It is obvious that for ν =.5 the volume of a material subjected to tensile forces will not change (dv = ), for ν <.5 the volume will increase (dv > ), while for ν >.5 it will decrease (dv < ). When a fabric is stretched in one direction, it tends to contract in the direction perpendicular to the direction of the stretch, Fig. 1b, 1c. The yarns in the direction of the tensile force are flattened out (extended), and in the orthogonal or nonloading direction, the yarns have a longer geometrical path to 'curve around'. Because there is no limiting force, the waviness (amplitude) of the yarn in the vertical direction of the force increases. The consequence to this is the dimension reduction of the fabric width. This phenomenon is called the Poisson effect. The Poisson s ratio, a measure of the Poisson effect, is the ratio of the relative contraction strain s to the related extension strain ε in the direction of the applied load. To determine the Poisson's ratio of fabrics, devices for measuring the tensile strength are used, and the coefficient is determined in the linear part of the diagram of the Hooke's law [1]. During the testing of the fabric to stretch, the initial length of the tested sample l is increased for Δl, and a final sample length of fabric is l. The initial width of the fabric sample b is decreased for Δb and the final sample width is b. The physical meaning of the Poisson's ratio ν is shown by the Eq. (3). The Relative contraction and extension strains have an opposite sign. (2) s l b b, b l l s. (3) The relative longitudinal strain (relative extension strain) ε and transverse strain (relative contraction strain) s is defined in the Eq. (4). l l 1% 1 1% l l. (4) b b s 1% 11% b b Due to the anisotropy of the fabric, the Poisson s ratio is being changed in the process of the extension of the fabric sample. 3 EXPERIMENTAL TESTING The experimental study was carried out by measuring the extension of woven fabrics samples under the action of the tensile force till rupture [11]. The tensile force acts on the samples that are cut at warp and weft direction. The values of the tensile force in relation to the relative extension were measured. For the extensions and tensile forces which act in the warp and weft direction, the corresponding contraction strains of woven fabrics were scanned. The Poisson's ratio of woven fabrics was calculated by using the testing results. Two different fabrics of a different raw material composition (, ) and of the same weave (plain weave) were available. The raw material and the structural properties of the tested fabrics are shown in Tab. 1. Table 1 Structural characteristics of the tested samples Warp direction Weft direction Fabric structure Fiber Yarn count Linera density Fiber Linera density Mass per unit Thickness, t composition (tex) (cm 1 Yarn count (tex) ) composition (cm 1 ) area (g/m 2 ) (mm) Plain Cotton Cotton Plain Wool Wool TECHNICAL JOURNAL 11, 3(217), 1116
3 The yarn count was determined by the gravimetric method according to the standard ISO 26:1994. The number of threads per unit length was tested according to the standard ISO :1984. The standard ISO 584:1996 describes a method for the determination of the thickness of the fabric. Before testing all samples were conditioned under the conditions of the standard atmosphere (relative air humidity 65 ± 2 %, at a temperature of 2 ± 2 C). Standard samples with the dimensions of 3 5 mm were cut and clamped in clamps of the tensile tester at a distance of l =2 mm and subjected to a uniaxial tensile load till rupture. The pulling speed of clamps is 1 mm/min. The samples were cut in the weft direction (φ = ) and warp direction (φ = 9 ). Three tests were done on the tensile tester for each mentioned cutting direction of the sample. The tensile properties of all samples were tested in accordance with the standard ISO ISO :28 by using the strip method for measuring the fabric strength on the tensile strength tester Textechno Statimat M. This tensile tester is an automatic, microprocessorcontrolled instrument operating on the principle of constant deformation speed, Fig. 2. Textechno sample sync on/off Figure 2 Schematic view of the experiment CAMERA SOFTWARE STATIMAT M SOFTWARE For an accurate recording and measurement of the spatial deformation of fabric, a 1x1 grid pattern was mounted on the tensile tester immediately behind the test specimen; the whole process of drawing the specimen till rupture was recorded by the Panasonic NVGS5 Digital Video Camera placed on a tripod in front of the device. The digital video camera had the resolution of pixels, and a recording speed of N sl=25 frames/s, and was connected to the computer via an IEEE 1394 (FireWire) interface. The horizontal distance between the camera and the sample was such that 1 mm on the grid amounted to 1 pixels on the picture. Two sources of white light which mutually closed the angle of 9 were used for measuring. The number of images N at a certain extension is: l 6 N Nsl. (5) 1 v The tensile tester and the camera were connected to a special assembly with a simultaneous on/off which fully ensured the exactness of the video recording of the entire process of stretching the fabric to rupture. The width of each sample was measured in three spots (1/4, 2/4 and 3/4 of the length and width of the sample). The transverse strain was obtained after all samples were recorded by camera, and the mentioned grid pattern enabled a fast and accurate editing of the footage processed by the software package Adobe Premiere created for this purpose which specified the spatial deformation of samples on the basis of shifting in the direction of the x and yaxis. 3.1 Overview of testing results The diagrams (Fε) of mean values of the test results of the action of the tensile force F and the corresponding longitudinal strain (extension) ε for the samples that are cut in the weft and warp direction are shown in Fig F (N) 3 F (N) a) b) Figure 3 Tensile forceelongation diagram (Fε) till rupture: a) when the force acts in the weft direction, b) when the force acts in the warp direction TEHNIČKI GLASNIK 11, 3(217),
4 3.2 Determination of Poisson's ratio The fabric sample width is b = 5 pixels, which is equivalent to b = 5 mm. When reading the value of the fabric width, after the effect of the force, the relative transverse strain is calculated by using the Eq. (4). The contraction of fabric occurs in the transverse direction, i.e. in the direction which is perpendicular to the direction of stretching. Due to this phenomenon, there is a loss of the rectangular shape of the sample, i.e. there is a contraction of the fabric sample. The relation between the continuous change of the relative contraction s (%) of the sample and its relative extension when a force acts on the samples that are cut in the weft direction is shown in Fig. 4a by a characteristic curve. Fig. 4b shows a characteristic curve of the relative contraction of the sample in relation to its relative extension when the force acts on samples that are cut in the warp direction. When a force acts on samples that are cut in the weft and warp direction, at the same relative extension ε, fabric has a higher relative contraction s than fabric, Fig. 4. When the force acts in the weft direction, at a relative extension ε = 1%, the lateral contraction for the fabric is s = 12.56% and for fabric s = 7.57 %. The lateral contraction of fabric is 66% higher than the contraction of fabrics for ε = 1%. When force acts in the warp direction, at a relative extension ε = 15.5%, the lateral contraction for fabric is s = 17.47% and for fabric s = 9.12%. The lateral contraction of fabric is 92% higher than the contraction of fabric for ε = 15.5%. Both fabrics have a bigger extension and contraction when the force acts in the warp direction s (%) 68 s (%) a) b) Figure 4 Diagram of the relative contraction of the fabric s (%): a) when the force acts in the weft direction, b) when the force acts in the warp direction 2 From the diagrams in Fig. 4 it is evident that fabric contractions are small at the beginning of stretching. After that, with the increase of stretching, the values of fabric contractions also increase. According to the Eq. (3) and based on the experimental values of the relative contraction s and relative extension ε from Fig. 4, the values of the Poisson s ratio v are calculated when the force acts on the samples that are cut in the weft and warp direction. Fig. 5a shows a curve of the values of the Poisson s ratio v in relation to its relative extension when the force acts on the samples that are cut in the weft direction and Fig. 5b shows the values in the warp direction a) b) Figure 5 Poisson s ratio v of the fabric: a) when the force acts in the weft direction, b) when the force acts in the warp direction 14 TECHNICAL JOURNAL 11, 3(217), 1116
5 The shape of the Poisson s ratio curve of the woven fabric is the result of the internal interactions in the fabric. The shape of the Poisson s ratio (Fig. 5) affected by the changes in the value of the relative contraction of the fabric are shown in Fig. 4. The Poisson s ratio curve consists of two zones. The first zone includes the area from the beginning to the highest peak of the curve. When a force acts in the weft direction, the highest value of the Poisson s ratio for the fabric ν = 1.39 is where the relative extension ε is between 6 and 6.5%, and for fabric ν =.88 is where ε is between 5.5 and 6%, Fig. 5a. When a force acts in the warp direction, the highest value of the Poisson s ratio for the fabric ν = 1.18 is where the relative extension ε is between 14 and 14.5%, and for fabric ν =.68 is where ε is between 9.5 and 1%, Fig. 5b. Both fabrics have a higher value of the Poisson s ratio when the force acts in the weft direction. Cotton fabric has a higher value of the Poisson s ratio than fabric for each value of the extension. When the force acts in the weft direction, at a relative extension ε = 6 %, the value of the Poisson s ratio for fabric is 62% higher than the Poisson s ratio for fabrics. When the force acts in the warp direction, at a relative extension ε = 6 %, the value of Poisson s ratio for fabric is 52% higher than the Poisson s ratio for fabrics. The second zone is from the highest peak of the curve to the end of stretching, i.e. it is interrupted. In this zone, the curve of the Poisson s ratio decreases and it represents the end of the lateral contraction despite the stretching of the fabric sample. After considering the equation of the Poisson s ratio, the relative contraction becomes a constant when the lateral contraction of the woven fabric is completed. Furthermore, the sample is still stretching for the value ε. Therefore, the equation of the Poisson s ratio takes on a new form, which is the general form of the reciprocal function. Mathematically, the limit of this equation is zero. In practice, due to the break of the sample, this condition never occurs. However, taking into account the significance of the Poisson s ratio that represents the ratio between the transverse and longitudinal deformation of the material, if the transverse deformation does not take place in this ratio, the Poisson s ratio has no practical significance. The ending of the lateral contraction of a woven fabric can occur for two reasons. Firstly, due to the termination of the flattening crimp of yarn in the direction of the stretching fabric and secondly, because of the structure of the fabric. If there is a possibility of a further contraction of fabric, it can not continue taking place because there is no continued existence of space between the neighboring threads in the fabric, so there can be no contraction of the fabric. Note: This research was presented at the International Conference MATRIB 217 (29 June  2 July 217, Vela Luka, Croatia). 4 CONCLUSION Due to the anisotropy of woven fabrics, the Poisson's ratio is not constant, but varies with each fabric extension. The behavior and shape of the Poisson s ratio curve of the coated fabric that is subjected to the tensile force mostly depends on its behavior in a direction perpendicular to the extension. The Poisson s ratio values depend on the number of coatings applied to the raw fabric. The shape of the Poisson s ratio curve for woven fabrics is a result of the internal interactions in the coated and raw fabrics. A change in the values of the relative contraction of coated fabrics affects the shape of the Poisson s ratio curve. When the force acts on samples that are cut in the weft direction, the Poisson's ratio assumes the maximum value at a relative extension of fabrics between 6 and 6.5%, and for fabrics between 5 and 5.5%. When the force acts on the samples that are cut in the warp direction, the Poisson s ratio assumes the maximum value at a relative extension of fabrics between 14 and 14.5%, and between 9.5 and 1% for fabrics. In the weft and warp direction, the values of the Poisson s ratio of fabrics are higher than the Poisson s ratio of fabrics at the same relative extension. Because of the anisotropy of fabrics, the Poisson s ratio is not constant. It is changing with each elongation of the woven fabric. The behavior and form of the curve of the Poisson s ratio of the woven fabric which is exposed to tensile force, i.e. elongation, mainly depends on the behavior of the fabric in a direction perpendicular to the elongation. First, the Poisson s ratio increases nonlinearly and after having reached the peak value, it decreases. These two zones represent two different processes in the deformation of the fabric. The first zone represents the way of the lateral contraction because of the longitudinal stretching. The second zone shows the termination of the lateral contraction of the woven fabric and the fabric is stretching without any further contractions. 5 REFERENCES [1] Kovar, R.; Gupta, B. S. Study of the Anisotropic Nature of the Rupture Properties of a Plain Woven Fabric. // Textile Research Journal, 79, 6(29), pp [2] Peirce, F. T. The geometry of cloth structure. // Journal of the Textile Institute, 28, (1937), T45T96. [3] Kilby, W. F. Planar Stressstrain Relationship in Woven Fabrics. // Journal of the Textile Institute, 54, (1963), pp [4] Lloyd, D. W. et al. An Examination of a "Wide jaw" Test for the Determination of Fabric Poisson Ratio. // Journal of the Textile Institute, 68, 9(1977), pp [5] Bao, L. et al. Error Evaluation in Measuring the Apparent Possion s Ratios of Textile Fabrics by Uniaxial Tensile Test. // Sen i Gakkaishi, 53, 1(1997), pp TEHNIČKI GLASNIK 11, 3(217),
6 [6] Basset, R. J. et al. Experiment Methods for Measuring Fabric Mechanical Properties: a Review and Analysis. // Textile Research Journal, 69, 11(1999), pp [7] Sun, H. On the Poisson's ratios of a woven fabric. // Composite Structures, 68, 4(25), pp [8] Zheng, J. Measuring Technology of the Anisotropic Tensile Properties of Woven Fabrics. // Textile Research Journal, 78, 12(28), pp [9] Giroud, J. P. Poisson's Ratio of Unreinforced Geomembranes and Nonwoven Geotextiles Subjected to Large Strains. // Geotextiles and Membrane, 22, (24), pp [1] Nazanin, E. S. et al. Effect of Fabric Structure and Weft Density on the Poisson s Ratio of Worsted Fabric. // Journal of Engineered Fibers and Fabrics, 8, 2(213), pp [11] Penava, Ž. et al. Investigation of warp and weft takeup influence on Poisson's ratio of woven fabric. // Tekstil, 63, 78(214), pp Authors contacts: Željko PENAVA University of Zagreb, Faculty of Textile Technology, Prilaz B. Filipovića 28a, 1 Zagreb, Croatia Diana ŠIMIĆ PENAVA University of Zagreb, Faculty of Civil Engineering, Kačićeva 26, 1 Zagreb, Croatia Željko KNEZIĆ University of Zagreb, Faculty of Textile Technology, Prilaz B. Filipovića 28a, 1 Zagreb, Croatia 16 TECHNICAL JOURNAL 11, 3(217), 1116
CHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationPullout Tests of Geogrids Embedded in Noncohesive Soil
Archives of HydroEngineering and Environmental Mechanics Vol. 51 (2004), No. 2, pp. 135 147 Pullout Tests of Geogrids Embedded in Noncohesive Soil Angelika Duszyńska, Adam F. Bolt Gdansk University of
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationLab Exercise #3: Torsion
Lab Exercise #3: Prelab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationPrecise Measurement of Tension on Curvature Elastic Shells
Precise Measurement of Tension on Curvature Elastic Shells Marzie Aghajani, Mohammad Amani Tehran, PhD, Ali Asghar Asgharian Jeddi, PhD Amir Kabir University, Tehran IRAN Correspondence to: Mohammad Amani
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationChapter 13 ELASTIC PROPERTIES OF MATERIALS
Physics Including Human Applications 280 Chapter 13 ELASTIC PROPERTIES OF MATERIALS GOALS When you have mastered the contents of this chapter, you will be able to achieve the following goals: Definitions
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationMECHANICAL PROPERTIES OF SOLIDS
Chapter Nine MECHANICAL PROPERTIES OF SOLIDS MCQ I 9.1 Modulus of rigidity of ideal liquids is (a) infinity. (b) zero. (c) unity. (d) some finite small nonzero constant value. 9. The maximum load a wire
More informationINDUSTRIAL FORMING SIMULATION OF MULTILAYERED UD NONCRIMPFABRICS. 13. LSDYNA FORUM, , BAMBERG.
Sebastian Kreissl, Thomas Senner, Arnulf Lipp, Josef Meinhardt. INDUSTRIAL FORMING SIMULATION OF MULTILAYERED UD NONCRIMPFABRICS. 13. LSDYNA FORUM, 07.10.2014, BAMBERG. OUTLINE. BMW i. Production Process
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationFinite Element Modeling of an Aluminum Tricycle Frame
Finite Element Modeling of an Aluminum Tricycle Frame A. Rodríguez, B. Chiné*, and J. A. Ramírez Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationA MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE
A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE 2014 A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS
More informationReteach 23. Graphing Linear Functions. 22 Holt Algebra 2. Name Date Class
3 Graphing Linear Functions Use intercepts to sketch the graph of the function 3x 6y 1. The xintercept is where the graph crosses the xaxis. To find the xintercept, set y 0 and solve for x. 3x 6y 1
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationUnified Quiz M4 May 7, 2008 M  PORTION
9:0010: 00 (last four digits) 32141 Unified Quiz M4 May 7, 2008 M  PORTION Put the last four digits of your MIT ID # on each page of the exam. Read all questions carefully. Do all work on that question
More informationDEVELOPMENT OF AN EXPERIMENTAL AUTOMATIC WET SPINNING MACHINE
14 th AUTEX World Textile Conference May 26 th to 28 th 2014, Bursa, Turkey DEVELOPMENT OF AN EXPERIMENTAL AUTOMATIC WET SPINNING MACHINE P.WEISSER 1, A. HEKMATI 1, G. BARBIER 1, JY. DREAN 1 1 ENSISALaboratoire
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationASSESSING THE QUALITY OF NEURAL MODELS USING A MODEL OF FLOW CHARACTERISTICS OF FABRICS AS AN EXAMPLE
ASSESSING THE QUALITY OF NEURAL MODELS USING A MODEL OF FLOW CHARACTERISTICS OF FABRICS AS AN EXAMPLE Magdalena Tokarska Department for Automation of Textile Processes, Technical University of Łódź Zeromskiego
More informationBeam Bending Stresses and Shear Stress
Beam Bending Stresses and Shear Stress Notation: A = name or area Aweb = area o the web o a wide lange section b = width o a rectangle = total width o material at a horizontal section c = largest distance
More informationDesign of reinforced concrete sections according to EN and EN
Design of reinforced concrete sections according to EN 199211 and EN 19922 Validation Examples Brno, 21.10.2010 IDEA RS s.r.o. South Moravian Innovation Centre, U Vodarny 2a, 616 00 BRNO tel.: +420511
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationSTRENGTH OF MATERIALS 140AU0402 UNIT 1: STRESS STRAIN DEFORMATION OF SOLIDS
UNIT 1: STRESS STRAIN DEFORMATION OF SOLIDS Rigid and Deformable bodies Strength, Stiffness and Stability Stresses; Tensile, Compressive and Shear Deformation of simple and compound bars under axial load
More informationMECHANICS OF SOLIDS Credit Hours: 6
MECHANICS OF SOLIDS Credit Hours: 6 Teaching Scheme Theory Tutorials Practical Total Credit Hours/week 4 0 6 6 Marks 00 0 50 50 6 A. Objective of the Course: Objectives of introducing this subject at second
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationIdentification of the plastic zone using digital image correlation
M. Rossi et alii, Frattura ed Integrità Strutturale, 3 (4) 55557; DOI:.3/IGFESIS.3.66 Focussed on: Fracture and Structural Integrity related Issues Identification of the plastic zone using digital image
More informationAnalysis of Thermal Stress in Fatigue Fracture Specimen using Lockin Thermography
Analysis of Thermal Stress in Fatigue Fracture Specimen using Lockin Thermography WonTae Kim*, ManYong Choi**, JungHak Park** * Major of Biomechanical Engineering, Kongju National University, Chungnam,
More informationChapter 5. Vibration Analysis. Workbench  Mechanical Introduction ANSYS, Inc. Proprietary 2009 ANSYS, Inc. All rights reserved.
Workbench  Mechanical Introduction 12.0 Chapter 5 Vibration Analysis 51 Chapter Overview In this chapter, performing free vibration analyses in Simulation will be covered. In Simulation, performing a
More informationTangential or Shearing
UNITII PROPERTIES OF MATTER INTRODUCTION Elasticity is a branch of Physics which deals with the elastic property of materials. When an external force is applied to a body, there will be some change in
More informationMidterm 2 PROBLEM POINTS MAX
Midterm 2 PROBLEM POINTS MAX 1 30 2 24 3 15 4 45 5 36 1 Personally, I liked the University; they gave us money and facilities, we didn't have to produce anything. You've never been out of college. You
More informationBy drawing Mohr s circle, the stress transformation in 2D can be done graphically. + σ x σ y. cos 2θ + τ xy sin 2θ, (1) sin 2θ + τ xy cos 2θ.
Mohr s Circle By drawing Mohr s circle, the stress transformation in D can be done graphically. σ = σ x + σ y τ = σ x σ y + σ x σ y cos θ + τ xy sin θ, 1 sin θ + τ xy cos θ. Note that the angle of rotation,
More informationCombined Stresses and Mohr s Circle. General Case of Combined Stresses. General Case of Combined Stresses con t. Twodimensional stress condition
Combined Stresses and Mohr s Circle Material in this lecture was taken from chapter 4 of General Case of Combined Stresses Twodimensional stress condition General Case of Combined Stresses con t The normal
More informationJournal of Power Sources
Journal of Power Sources 190 (2009) 92 102 Contents lists available at ScienceDirect Journal of Power Sources journal homepage: www.elsevier.com/locate/jpowsour Characterisation of mechanical behaviour
More informationTHEME A. Analysis of the elastic behaviour of La Aceña archgravity dam
THEME A Analysis of the elastic behaviour of La Aceña archgravity dam Gjorgi KOKALANOV, Professor, Faculty of Civil Eng., Skopje, Republic of Macedonia Ljubomir TANČEV, Professor, Faculty of Civil Eng.,
More informationMATERIAL CHARACTERIZATION, VIBROACOUSTIC ANALYSIS AND MANUFACTURING OF TEXTILEREINFORCED COMPLEX 3D COMPOSITE STRUCTURES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MATERIAL CHARACTERIZATION, VIBROACOUSTIC ANALYSIS AND MANUFACTURING OF TEXTILEREINFORCED COMPLEX 3D COMPOSITE STRUCTURES Hufenbach, Werner*, Täger,
More informationFinite Element Analysis of Piezoelectric Cantilever
Finite Element Analysis of Piezoelectric Cantilever Nitin N More Department of Mechanical Engineering K.L.E S College of Engineering and Technology, Belgaum, Karnataka, India. Abstract Energy (or power)
More informationElastic moduli: Overview and characterization methods
Technical Review ITCME/ATCP Elastic moduli: Overview and characterization methods ATCP Physical Engineering www.atcpndt.com Authors: Leiliane Cristina Cossolino (Cossolino LC) and Antônio Henrique Alves
More informationTHE MECHANICAL BEHAVIOR OF ORIENTED 3D FIBER STRUCTURES
Lappeenranta University of Technology School of Engineering Science Degree Program in Computational Engineering and Technical Physics Master s Thesis Alla Kliuzheva THE MECHANICAL BEHAVIOR OF ORIENTED
More informationTMHL TMHL (Del I, teori; 1 p.) SOLUTION I. II.. III. Fig. 1.1
TMHL6 2040830 (Del I, teori; p.). Fig.. shows three cases of sharp cracks in a sheet of metal. In all three cases, the sheet is assumed to be very large in comparison with the crack. Note the different
More informationvs. Chapter 4: Standard Flows Chapter 4: Standard Flows for Rheology shear elongation 2/1/2016 CM4650 Lectures 13: Intro, Mathematical Review
CM465 Lectures 3: Intro, Mathematical //6 Chapter 4: Standard Flows CM465 Polymer Rheology Michigan Tech Newtonian fluids: vs. nonnewtonian fluids: How can we investigate nonnewtonian behavior? CONSTANT
More informationNumerical Modeling for Different Types of Fractures
umerical Modeling for Different Types of Fractures Xiaoqin Cui* CREWES Department of Geoscience University of Calgary Canada xicui@ucalgary.ca and Laurence R. Lines Edward S. Krebes Department of Geoscience
More informationInvestigation of Acrylic Resin Treatment and Evaluation of Cationic Additive Quality Impact on the Mechanical Properties of Finished Cotton Fabric
ISSN: 9 9, Volume, Issue, August 01 Investigation of Acrylic Resin Treatment and Evaluation of Cationic Additive Quality Impact on the of Finished Cotton Fabric Nasr Litim, Ayda Baffoun Abstract: Statistical
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationFINITE ELEMENT COUPLED THERMOMECHANICAL ANALYSIS OF THERMAL STRATIFICATION OF A NPP STEAM GENERATOR INJECTION NOZZLE
Proceedings of COBEM 2007 Copyright 2007 by ABCM 19th International Congress of Mechanical Engineering November 59, 2007, Brasília, DF FINITE ELEMENT COUPLED THERMOMECHANICAL ANALYSIS OF THERMAL STRATIFICATION
More informationStrain sensors based on bragg gratings
IMEKO 20 th TC3, 3 rd TC16 and 1 st TC22 International Conference Cultivating metrological knowledge 27 th to 30 th November, 2007. Merida, Mexico. Strain sensors based on bragg gratings K. Haase Hottinger
More informationSection 19.1: Forces Within Earth Section 19.2: Seismic Waves and Earth s Interior Section 19.3: Measuring and Locating.
CH Earthquakes Section 19.1: Forces Within Earth Section 19.2: Seismic Waves and Earth s Interior Section 19.3: Measuring and Locating Earthquakes Section 19.4: Earthquakes and Society Section 19.1 Forces
More informationBorehole Geophysics. Acoustic logging measurements
Acoustic logging measurements  Review of basic physics background  Concept of P and Swave measurements and logging tools  Tube waves  Seismic imaging  Synthetic seismograms  Field application examples
More informationGeometrydependent MITC method for a 2node isobeam element
Structural Engineering and Mechanics, Vol. 9, No. (8) 33 Geometrydependent MITC method for a node isobeam element PhillSeung Lee Samsung Heavy Industries, Seocho, Seoul 37857, Korea HyuChun Noh
More informationDesign and Analysis of Adjustable Inside Diameter Mandrel for Induction Pipe Bender
International Journal of Engineering Trends and Technology (IJETT) Volume0Number  Apr 0 Design and Analysis of Adjustable Inside Diameter Mandrel for Induction Pipe Bender S.Nantha Gopan, M.Gowtham J.Kirubakaran
More informationMechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total
Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationParametric analysis and torsion design charts for axially restrained RC beams
Structural Engineering and Mechanics, Vol. 55, No. 1 (2015) 127 DOI: http://dx.doi.org/10.12989/sem.2015.55.1.001 1 Parametric analysis and torsion design charts for axially restrained RC beams Luís F.A.
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationTwodimensional ternary locally resonant phononic crystals with a comblike coating
Twodimensional ternary locally resonant phononic crystals with a comblike coating YanFeng Wang, YueSheng Wang,*, and Litian Wang Institute of Engineering Mechanics, Beijing Jiaotong University, Beijing,
More informationThe Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar
The Influence of Discontinuities on Elastic and Mechanical Properties of Composite Materials Reinforced with Woven Carbon, Carbonkevlar and Kevlar DUMITRU BOLCU 1 *, MIHAELA SAVA 2, ALIN DINITA 3, COSMIN
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationBACKGROUND ANALYSIS OF THE BURST TEST GEOMETRY A NEW APPROACH ABSTRACT INTRODUCTION MEMBRANE ANALYSIS
ANALYSIS OF THE BURST TEST GEOMETRY A NEW APPROACH ABSTRACT John C. Strikwerda Associate Professor Computer Sciences Department University of WisconsinMadison John M. Considine Research General Engineer
More informationStiffness Matrices, Spring and Bar Elements
CHAPTER Stiffness Matrices, Spring and Bar Elements. INTRODUCTION The primary characteristics of a finite element are embodied in the element stiffness matrix. For a structural finite element, the stiffness
More informationWeek 10  Lecture Nonlinear Structural Analysis. ME Introduction to CAD/CAE Tools
Week 10  Lecture Nonlinear Structural Analysis Product Lifecycle Week 10 Requirements Portfolio Management Conceptual Design Product Engineering Manufacturing Engineering Simulation & Validation Build
More informationFINITEVOLUME SOLUTION OF DIFFUSION EQUATION AND APPLICATION TO MODEL PROBLEMS
IJRET: International Journal of Research in Engineering and Technology eissn: 3963 pissn: 3738 FINITEVOLUME SOLUTION OF DIFFUSION EQUATION AND APPLICATION TO MODEL PROBLEMS Asish Mitra Reviewer: Heat
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More information4. SHAFTS. A shaft is an element used to transmit power and torque, and it can support
4. SHAFTS A shaft is an element used to transmit power and torque, and it can support reverse bending (fatigue). Most shafts have circular cross sections, either solid or tubular. The difference between
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More informationAvailable online at ScienceDirect. Procedia Engineering 105 (2015 )
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 105 (015 ) 64 69 6th BSME International Conference on Thermal Engineering (ICTE 014) Numerical Study of SubNozzle Flows for
More informationEuroGeo4 Paper number 203 ANALYSIS OF MECHANICAL AND PHYSICAL PROPERTIES ON GEOTEXTILES AFTER WEATHERING EXPOSURE
Lodi, P.C., Bueno, B.S., Zornberg, J.G., and Correia, N.S. (8). Analysis of Mechanical and Physical Properties on Geotextiles after Weathering Exposure. Fourth European Geosynthetics Conference, EuroGeo4,
More informationNUMERICAL SIMULATIONS OF NAKAZIMA FORMABILITY TESTS WITH PREDICTION OF FAILURE
NUMERICAL SIMULATIONS OF NAKAZIMA FORMABILITY TESTS WITH PREDICTION OF FAILURE DMYTRO LUMELSKYJ 1, JERZY ROJEK 1, MAREK TKOCZ 2 Abstract. This paper presents results of numerical simulations of the Nakazima
More informationWrinkling Analysis of A Kapton Square Membrane under Tensile Loading
44th AIAA/ASME/ASCE/AHS Structures, Structural Dynamics, and Materials Confere 710 April 2003, Norfolk, Virginia AIAA 20031985 Wrinkling Analysis of A Kapton Square Membrane under Tensile Loading Xiaofeng
More informationPhysics 231 Lecture 23
Physics 31 Lecture 3 Main points of today s lecture: Gravitation potential energy GM1M PEgrav r 1 Tensile stress and strain Δ Y ΔL L 0 Bulk stress and strain: Δ V Δ P B Δ V Pressure in fluids: P ; Pbot
More informationFEM Modeling of a 3D Printed Carbon Fiber Pylon
FEM Modeling of a 3D Printed Carbon Fiber Pylon I. López G.*, B. Chiné, and J.L. León S. Costa Rica Institute of Technology, School of Materials Science and Engineering, Cartago, Costa Rica *Corresponding
More informationFlow and Transport. c(s, t)s ds,
Flow and Transport 1. The Transport Equation We shall describe the transport of a dissolved chemical by water that is traveling with uniform velocity ν through a long thin tube G with uniform cross section
More informationReliable Test Results
Intelligent testing Johannes J.Bührle  Agenda Reliable test results are a fundamental and highly topical aspect of materials testing. Using suitable examples we would like to show you how we view this
More informationDevelopment of GENOA Progressive Failure Parallel Processing Software Systems
NASA/CR 1999209404 Development of GENOA Progressive Failure Parallel Processing Software Systems Frank Abdi Alpha STAR Corporation, Long Beach, California Levon Minnetyan Clarkson University, Potsdam,
More informationL e c t u r e. D r. S a s s a n M o h a s s e b
The Scaled smteam@gmx.ch Boundary Finite www.erdbebenschutz.ch Element Method Lecture A L e c t u r e A1 D r. S a s s a n M o h a s s e b V i s i t i n g P r o f e s s o r M. I. T. C a m b r i d g e December
More informationOPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION
OPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION Luca Barbaresi, Federica Morandi, Juri Belcari, Andrea Zucchelli and Alice Speranza University
More informationDesign and Optimization of Piezoelectric DualMode MicroMirror
Design and Optimization of Piezoelectric DualMode MicroMirror Jichao Zhong, Xingguo Xiong, Zheng Yao, Junling Hu*, Prabir Patra* Department of Electrical and Computer Engineering, *Department of Mechanical
More informationFlexural Analysis of Deep Aluminum Beam
Journal of Soft Computing in Civil Engineering 1 (018) 7184 journal homepage: http://www.jsoftcivil.com/ Fleural Analysis of Deep Aluminum Beam P. Kapdis 1, U. Kalwane 1, U. Salunkhe 1 and A. Dahake
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationUnconventional DoubleCurrent Circuit for Deflection and Temperature Simultaneous Measurement
http://dx.doi.org/10.5755/j01.eee.21.1.6834 ELEKTRONIKA IR ELEKTROTECHNIKA ISSN 13921215 VOL. 21 NO. 1 2015 Unconventional DoubleCurrent Circuit for Deflection and Temperature Simultaneous Measurement
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationMODELING APPROACH OF MICROBUCKLING MECHANISM DURING CURE IN A CARBON EPOXY LAMINATE
MODELING APPROACH OF MICROBUCKLING MECHANISM DURING CURE IN A CARBON EPOXY LAMINATE Ch. Jochum 1, JC. Grandidier 2 & M. PotierFerry 1 1 Laboratoire de Physique et de Mécanique des Matériaux, UMR CNRS
More informationDamping of materials and members in structures
Journal of Physics: Conference Series Damping of materials and members in structures To cite this article: F Orban 0 J. Phys.: Conf. Ser. 68 00 View the article online for updates and enhancements. Related
More informationDynamic Mechanical Analysis of Solid Polymers and Polymer Melts
Polymer Physics 2015 Matilda Larsson Dynamic Mechanical Analysis of Solid Polymers and Polymer Melts Polymer & Materials Chemistry Introduction Two common instruments for dynamic mechanical thermal analysis
More information